Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Successfully reported this slideshow.

Like this presentation? Why not share!

- 01_INTRODUCTION_TO_FRACTURE_MECHANI... by Can Ozcan 3022 views
- Shear force and bending moment diagram by Muhammad Bilal 2375 views
- Forces acting on the beam with shea... by Taral Soliya 3323 views
- Lecture 11 shear stresses in beams by Deepak Agarwal 20489 views
- Structures and Materials- Outline a... by The Engineering C... 5456 views
- fracture mechanics presentation by M Shahid Khan 3153 views

No Downloads

Total views

2,679

On SlideShare

0

From Embeds

0

Number of Embeds

4

Shares

0

Downloads

173

Comments

0

Likes

5

No embeds

No notes for slide

- 1. REVA UNIVERSITY A PRESENTATION ON FRACTURE MECHANICS Under Guidance of Prof: SHIVASHARANAYYA SWAMY Presented by BEERAPPA RU14MMD02
- 2. FRACTURE MECHANICS
- 3. CONTENTS • Introduction • An atomic view of fracture • Stress concentration effect of flaws • The Griffith energy balance • Modified Griffith equation • The energy release rate • References
- 4. INTRODUCTION • A fracture is the separation of an object or material into two or more pieces under the action of stress. • Fracture mechanics is the field of mechanics concerned with the study of the propagation of cracks in materials. It uses methods of analytical solid mechanics to calculate the driving force on a crack and those of experimental solid mechanics to characterize the material's resistance to fracture. Three modes of fracture • Mode 1 denotes a symmetric opening(opening mode) • Mode 2 denotes an antisymmetric separation(in plane shear mode) • Mode 3 denotes an antisymmetric separation(tearing mode)
- 5. AN ATOMIC VIEW OF FRACTURE • A material fractures when sufficient stress and work are applied on the atomic level to break the bonds that hold atoms together. • The bond strength is supplied by the attractive forces between atoms. • Figure 1. shows schematic plots of the potential energy and force versus separation distance between atoms. • The equilibrium spacing occurs where the potential energy is at a minimum. • A tensile force is required to increase the separation distance from the equilibrium value, this force must exceed the cohesive force to sever the bond completely.
- 6. Potential energy and force vs the separation distance between atoms
- 7. • The bond energy is given by (1) where xo is the equilibrium spacing and P is the applied force. • It is possible to estimate the cohesive strength at the atomic level by idealizing the interatomic force-displacement relationship as one half the period of a sine wave: (2) • where the distance λ is defined in Figure 1 For the sake of simplicity, the origin is defined at xo. For small displacements, the force-displacement relationship is linear; (3)
- 8. • Bond stiffness is given by (4) • Multiplying both sides of this equation by the number of bonds per unit area and the gage length, xo, converts k to Young’s modulus E and Pc to the cohesive stress σc. Solving for σc gives (5) or (6) Lamda is assumbed to be approximately equal to the atomic spacing.
- 9. • The surface energy can be estimated as follows (7) • The surface energy per unit area, Ys, is equal to one half the fracture energy because two surfaces arc created when a material fractures. Substituting Eq (5) into Eq. (7) and solving for σc gives (8)
- 10. STRESS CONCENTRATION EFFECT OF FLAWS • The derivation in the previous section showed that the theoretical cohesive strength of a material is approximately E/π. • Experiments by Leonardo da Vinci, Griffith. and others indicated that the discrepancy be tween the actual strengths of brittle materials and theoretical estimates was due to flaws in these materials. • Fracture cannot occur unless the stress at the atomic level exceeds the cohesive strength of the material. • Inglis [I], who analyzed elliptical holes in flat plates. His analyses included an elliptical hole 2a long by 2b wide with an applied stress perpendicular to the major axis of the ellipse (see Fig. 2). • He assumed that the hole is not influenced by the plate boundary; i.e., the plate width >> 2o and the plate height >>>2b. The stress at the tip of the major axis (Point A) is given by
- 11. (9) • As the major axis, a , increases relative to b, the elliptical hole begins to take on the appearance of a sharp crack. For this case, Inglis found it more convenient to express Eq. (9)in terms of the radius of curvature p: (10) where (11) • When a >> b, Eq. (10) becomes (12)
- 12. Fig 2 Elliptical hole in a plate • Inglis showed that Eq. (12) gives a good approximation for the stress concentration due to a notch that is not elliptical except at the tip. • By substituting ρ=xo into Equation(12), we obtain an estimate of the local stress concentration at the tip of an atomically sharp crack, (13)
- 13. • If it is assumed that fracture occurs when Equation (13) can be set equal to Equation (8), resulting in the following expression for the remote stress at failure: (14) • Gehlen and Kanninen [3] obtained similar results from a numerical simulation of a crack in a two dimensional lattice, where discrete “atoms” were connected by nonlinear springs: (15) Where α is a constant.
- 14. THE GRIFFITH ENERGY BALANCE • According to the First law of Thermodynamics, when a system goes from a non equilibrium state to equilibrium, there will be a net decrease in energy. • A crack can form only if such a process causes the total energy to decrease or remain constant. Thus the critical conditions for fracture can be defined as the point where crack growth occurs under equilibrium conditions, with no net change in total energy. • Consider a plate subjected to a constant stress, a, which contains a crack 2a long(Fig.3). • Assume that the plate width>> 2a and that plane stress conditions prevail. In order for this crack to increase in size, sufficient potential energy must be available in the plate to overcome the surface energy of the material. The Griffith energy balance for an incremental increase in the crack area dA,under equilibrium conditions, can be expressed in the following way:
- 15. (16) or (17) Where E= total energy Π= potential energy supplied by the internal strain energy and external forces Ws= work required to create new surfaces • For the cracked plate illustrated in Figure 3, Griffith used the stress analysis of Inglis to show that (18) Where Πo is the potential energy of an uncracked plate and B is the plate thickness.
- 16. Fig.3 through-thickness crack in an infinitely wide plate subjected to a remote tensile stress. • Since the formation of a crack requires the creation of two surfaces, Ws is given by (19) Where γs is the surface energy of the material. Thus (20) Or (21)
- 17. • Equating eq(20) and eq(21) solving for fracture stress gives (22) • Fig 4 A penny-shaped (circular) crack embedded in a solid subjected to a remote tensile stress. • The Griffith approach can be applied to other crack shapes. For example, the frature stress for a penny-shaped flaw embedded in the material is given by (23) where a is the crack radius and ν is Poisson’s ratio
- 18. MODIFIED GRIFFITH EQUATION • Irwin [4] and Orowan [5] independently modified the Griffith expression to account for materialsnthat are capable of plastic flow. The revised expression is given by (24) where γp is the plastic work per unit area of surface created and is typically much larger than γs . FIGURE 5. A sharp microcrack at the tip of a macroscopic crack.
- 19. • Although Irwin and Orowan originally derived Equation for metals, it is possible to generalize the Griffith model to account for any type of energy dissipation: (25) where wf is the fracture energy, which could include plastic, viscoelastic, or viscoplastic effects, depending on the material.
- 20. Fig (a) Crack propagation in brittle material,
- 21. Crack propagation in various types of materials, with the corresponding fracture energy. (b)quasi-brittle elastic-plastic material and, (c)brittle material with crack meandering and branching.
- 22. THE ENERGY RELEASE RATE • In 1956, Irwin proposed an energy approach for fracture that is essentially equivalent to the Griffith model. Irwin defined an energy release rate G, which is measure of the energy available for an increment of crack extension. (26) • G is the rate of change in potential energy with crack area. Since (j is obtained from the derivative of a potential. it is also called the crack extension force or the crack driving force. According to Eq. (20), the energy release rate for a wide plate in plane stress with a crack of length 2a (Fig. 3) is given by (27)
- 23. • Referring to the previous section, crack extension occurs when G reaches a critical value, i.e., (28) where Gc is a measure of the fracture toughness of the material. • The potential energy of an elastic body, Π, is defined as follows: (29) where U Is the strain energy stored in the body and F is the work done by external forces. • Consider a cracked plate that is dead loaded, as illustrated in Figure 2.7. Since the load is fixed at P, the structure is said to be load controlled. For this case and
- 24. Fig 7 Cracked plate at a fixed load P. Therefore and (30)
- 25. • When displacement is fixed , the plate is displacement controlled; F = 0 and Π = U. Thus (31) • It is convenient at this point to introduce the compliance, which is the inverse of the plate stiffness: (32) • By substituting Equation (32) into Equation (30) and Equation (31) it can be shown that (33) • for both load control and displacement control. Therefore, the energy release rate, as defined in Equation , is the same for load control and displacement control. Also (34)
- 26. Fig 8 . Cracked plate at a fixed displacement Δ.
- 27. • Equation(34) is demonstrated graphically in Figure 7(b) and Figure 8(b). In load control,a crack extension da results in a net increase in strain energy because of the contribution of the external force P: • When displacement is fixed, dF = 0 and the strain energy decreases: • where dP is negative. As can be seen in Figure 7(b) and Figure 8(b), the absolute values of these energies differ by the amount dPdΔ/2, which is negligible. Thus for an increment of crack growth at a given P and Δ.
- 28. IMPORTANCE OF FRACTURE MECHANICS • In material science,fracture mechanics is an important tool in improving the mechanical performance of mechanical components. • Fractography is widely used with fracture mechanics to understand the causes of failures . • Also the verify theoretical failure predictions with real life failures.
- 29. Application of Fracture Mechanics • Fracture mechanics can be used in different major areas: 1.designing 2.material selection and alloy development 3.determing the significance of defects 4.monitoring.control and failure analysis
- 30. REFERENCES • Third Editin of Fracture mechanics by T.L. Anderson
- 31. Thank you to all

No public clipboards found for this slide

Be the first to comment